**INTRODUCTION**

The family of mesoporous silica molecular sieves designated as M41S with pore diameters between 2.0 and 10 nm is of considerable interest for various applications [1]. Depending on the synthesis conditions, different phases may be obtained, such as the hexagonal 41, cubic 48, as well as the 50 lamellar compound. The MCM-48 molecular sieve has a cubic structure indexed in the Ia3d space group, having two continuous interpenetrating networks of chiral channels separated by an inorganic wall which follows a minimal surface gyroid. The three-dimensional open pore MCM-48 increases the number of interactions between reagents and catalytic sites, resulting in a higher activity and resistance to block pores [2-4]. The MCM-48 has proven to be eficient for applications in adsorption, catalysis, chromatography, and gas separation, among others.

The synthesis parameters used for mesoporous materials

**Optimization of MCM-48 synthesis using factorial design**

**(Otimização da síntese do MCM-48 usando planejamento fatorial)**

**(Otimização da síntese do MCM-48 usando planejamento fatorial)**

**A. R. do Nascimento****1*******_{, R. L. B. de A. Medeiros}**2**_{, M. A. de F. Melo}**1,2**_{, D. M. de A. Melo}**2,3**_{, M. J. B. de Souza}**4**

*1 _{Graduate Program in Chemical Engineering, Chemical Engineering Department, Technology Center; }*

*2*

_{Graduate Program in Science and Material Engineering, Center of Exact Sciences and Earth; }*3Graduate Program in Chemistry, Chemistry Department, Federal University of Rio Grande do Norte, *

*Lagoa Nova Campus, P.O. Box 1524, Natal, RN, Brazil 59078-970*

*4 _{Graduate Program in Chemical Engineering, Chemical Engineering Department, Center of Exact Sciences and }*

*Technology, Federal University of Sergipe, Av. Marechal Rondon, s/n, S. Cristóvão, SE, Brazil 49100-000*

**ale3ufs@yahoo.com.br*

**Abstract**

MCM-48 mesoporous materials were hydrothermally synthesized according to the 22_{ factorial design by varying the }

crystallization time and temperature of the synthesis gel, and characterized by means of X-ray diffraction analysis and
adsorption of N_{2}. In the crystallization temperature and time conditions used, speciic areas between 924 to 1102 m2_{.g}-1_{, }

pore volumes between 0.015 to 0.087 cm3_{.g}-1_{ and pore diameters between 3.2 to 4.0 nm were obtained. It was observed }

that for the syntheses performed at high temperature, the crystallization time should be reduced so that the material structure is formed.

**Keywords**: MCM-48, 22 factorial design, crystallization temperature and time.

**Resumo**

*O material mesoporoso MCM-48 foi sintetizado hidrotermicamente de acordo com o planejamento fatorial 22 _{, }*

*variando-se a temperatura e o tempo de cristalização do gel de síntese, e caracterizado através de análise por difração *
*de raios X e adsorção de N _{2}. Nas condições de temperatura e tempo de cristalização utilizadas, foram obtidas áreas *

*especíicas entre 924 a 1102 m2*

_{.g}-1_{, volumes de poros entre 0,015 a 0,087 cm}3.g-1 e diâmetros de poros entre 3,2 a 4,0*nm. Observou-se que, para as sínteses realizadas com temperatura elevada, deve-se reduzir o tempo de cristalização *
*para que a estrutura do material seja formada.*

**Palavras-chave**: MCM-48, planejamento fatorial 22, temperatura e tempo de cristalização.

can give different characteristics to the material, so the
choice of these parameters is of fundamental importance
for improving materials to be applied in different areas
[5]. The variations in temperature and reaction time
inluence the speciic area, volume and pore diameter.
The factorial design 2n_{ is used to obtain the best operating }

hydrothermal synthesis parameters of time and temperature in the formation of MCM-48, especially in the speciic area, volume and pore diameter.

**EXPERIMENTAL**

*Experimental design*: the full factorial design 22_{ with }

triplicate central point was used to build the matrix of experiments. Seven experiments were performed, three of them repetitions at the central point. Table I shows the variables used in the design and combinations of upper (+) and lower (–) levels, and central point (0) for the variables used. The coeficients of the mathematical model were obtained after the analysis of the effects. The surfaces responses were obtained after evaluation of the mathematical model by ANOVA (analysis of variance).

*Hydrothermal synthesis of MCM-48*: the preparation
of solid mesoporous MCM-48 type was performed using
the hydrothermal method, following procedure described
in [19] with the necessary adaptations, as reported in [20].
TEOS (Sigma-Aldrich) were used as the source of silicon,
NaOH (Vetec) as the source of sodium, CTMABr (Vetec)
as structural conductors and distilled water as the solvent.
The molar chemical composition of the synthesis gel was
obtained using the following formula: 0.25Na2O-1SiO2
-0.55CTMABr-100H2O. The general synthesis procedure
consisted in preparing a solution, without pH control,
containing the driver structure and sodium hydroxide in the
amount of water required for the synthesis. The solution
was subjected to stirring at 50 °C to solubilize the structural
conductors. The source of silicon (TEOS) was added and the
solution remained stirring at 50 °C for 40 min. The material
was transferred to a Telon autoclave, which was jacketed
by stainless steel. The reaction temperature and time were
used according to the matrix of experiments for
MCM-48 synthesis shown in Table I. The obtained material was
calcined under synthetic air at 550 °C for 2 h.

*Characterization*: the synthesized samples were

analyzed by X-ray diffraction (Shimadzu XRD, 7000) and the angle range used between 1° and 10° in order to verify the formation of hexagonal mesoporous structure; physical adsorption characterization with N2 (Quantachrome Nova

2000) was used to evaluate the speciic area (BET method), such as volume and pore size distribution (BJH method).

The material presented better textural characteristics in that design was synthesized and used as adsorbent by [20] for the capture of CO2.

**RESULTS AND DISCUSSION**

Figs. 1 and 2 show the X-ray diffraction (XRD) patterns of the calcined and uncalcined synthesized samples, obtained from the experimental matrix of Table I. The temperature adversely interacts with the crystallization time of the synthesis gel; this means that when moving from higher levels of both temperature and time simultaneously (150 °C for 72 h), there is no MCM-48 structure formation. Therefore, for high-temperature synthesis, one should reduce the reaction time so that the material structure is formed. In the syntheses performed at lower temperature levels and higher and lower levels of crystallization time, there was MCM-48 structure formation. The textural properties of synthesized samples such as surface area, pore volume and diameter, mesoporous structure parameter and wall thickness are shown in Table II.

Tables III, IV and V show the estimated effects for
each factor (crystallization temperature and time) and
interactions, as well as the p-value and the coeficients
for constructing the mathematical model response to the
speciic area, pore diameter and pore volume, respectively.
For the variable to be considered statistically signiicant,
p-value should be below 0.05 (1-0.95) [6]. The p-values
obtained (Table III) show that the variables of crystallization
temperature and time did not signiicantly inluence the
increase in the speciic area of the material and other factors
can affect this parameter such as the stoichiometric amount
of reagents. Under the crystallization temperature and time
conditions used, speciic areas were obtained between
924 to 1102 m2_{.g}-1_{. According to the data in Table IV, it is }

observed that the p-values obtained are below 0.05, showing that the temperature and crystallization time variables used signiicantly inluence the pore diameter of the synthesized materials. According to the data in Table V, it is observed that the p-values were greater than 0.05, showing that the variables of crystallization time and temperature did not signiicantly increase the pore volume of the material, as occurred for the speciic area parameter.

Through the straight linear adjustment shown in Table IV, a mathematical model for the pore diameter was obtained (Equation A). According to this model, the optimal temperature and crystallization time values of the gel for further synthesis of MCM-48 can be obtained from the signiicant pore diameter. Its application allows for selecting the combination of maximized levels in getting the best response for every situation.

Dp = 3.546 + 0.122.t + 0.112.T + 0.503.t.T (A)

where, t represents the time in h and T the temperature in °C. To analyze the adjustment or reliability of the mathematical model, an analysis of variance (ANOVA) was conducted which shows the p-values (Table VI) for each variable

Experiment Temperature (°C) Time (h)

I 100 (–) 24 (–)

II 150 (+) 24 (–)

III 100 (–) 72 (+)

IV 150 (+) 72 (+)

Central point 125 (0) 48 (0)

Central point 125 (0) 48 (0)

Central point 125 (0) 48 (0)

Figure 1: XRD patterns of samples related to experiments I and II, crystallization at 100 and 150 °C during 24 h, and experiments III and IV, crystallization at 100 and 150 °C during 72 h.

*[Figura 1: Difratogramas de raios X das amostras referentes aos ensaios I e II, cristalização a 100 e 150 °C por 24 h, e aos *
*ensaios III e IV, cristalização a 100 e 150 °C por 72 h.]*

0

0

**2**q** (degree)**

**In**

**te**

**s**

**ity**

** (a**

**.u**

**.)**

**In**

**te**

**s**

**ity**

** (a**

**.u**

**.)**

**2**q** (degree)**

**2**q** (degree)**

**2**q** (degree)**
4.2k

4.2k 3.0k

3.0k 1.8k

1.8k

600.0

600.0

3.6k

3.6k 2.4k

2.4k 1.2k

1.2k

0.0

0.0

0

0 4

4

4

4

8

8

8

8

2

2

2

2 6

I Calcined

III Calcined

II Calcined

IV Calcined I UnCalcined

III UnCalcined

II UnCalcined

IV UnCalcined

6

6

6 10

10

10

10

**a)**

**c)**

**b)**

**d)**

Experiment a_{0} (nm) S_{BET} (m2.g-1) Vp (cm3.g-1) Dp (nm) W (nm)

I 8.42 1008 0.026 4.03 0.71

II 8.88 924 0.087 3.25 1.23

III 8.64 1010 0.015 3.27 1.16

V 8.20 1080 0.068 3.25 1.06

VI 8.26 1102 0.062 3.27 1.08

VII 8.20 1067 0.065 3.26 1.08

Table II - Textural properties of MCM-48 samples.

*[Tabela II - Propriedades texturais das amostras de MCM-48.]*

*Legend: a0 - lattice parameter of mesoporous structure (a0 = d211√6), SBET - speciic area, Vp - pore volume, Dp - pore diameter, *
*W - wall thickness.*

Factor Effect Standard deviation p-value Coeficient

Average 1167.457 49.673 0.00185 1167.457

(1) Time (h) 402.205 157.081 0.12464 201.103

(2) Temperature (°C) 215.806 157.081 0.30320 107.903

1 with 2 300.225 157.081 0.19613 150.113

Table III - Estimated effects of variables for the speciic area parameter.

used for pore diameter results, which showed p-values <0.05. With respect to the value of p, it can be seen that the model is statistically signiicant, showing that the time and temperature exert signiicant inluence on the MCM-48 synthesis.

After adjusting the model to the values of the experiment

results, the response surfaces were obtained in order to verify the conditions for obtaining the MCM-48 with high pore diameter. The response surfaces were constructed for all possible combinations of the variables of temperature and crystallization time. A graph of the optimized response surface Figure 2: XRD patterns of samples related to experiments V,

VI and VII, crystallization at 125 °C during 48 h.

*[Figura 2: Difratogramas de raios X das amostras referentes *
*aos ensaios V, VI e VII, cristalização a 125 °C por 48 h.]*

1000

**In**

**te**

**n**

**s**

**ity**

** (a**

**.u**

**.)** 800

600

400

200

0 0

**2**_{q}** (degree)**

6 6 6

3 90 3 90 3 9

Table VI - Analysis of variance (ANOVA) for setting the mathematical model for the pore diameter parameter.

*[Tabela VI - Análise da variância (ANOVA) para o ajuste do modelo matemático para o parâmetro diâmetro de poros.]*

Source of variance Quadratic sum Degree of freedom Mean square p-value

(1) Time (h) 0.1744 1 0.1744 0.00021

(2) Temperature (°C) 0.1829 1 0.1829 0.00020

1 with 2 0.0000 1 0.0000 0.95098

Pure error 0.000073 2 0.000037

Total 0.4972 5

Factor Effect Standard deviation p-value Coeficient

Average 3.546 0.0023 0.000000 3.546

(1) Time (h) 0.243 0.0061 0.000618 0.122

(2) Temperature (°C) 0.225 0.0061 0.000722 0.112

1 with 2 1.006 0.0061 0.000036 0.503

Table IV - Estimated effects of variables for the pore diameter parameter.

*[Tabela IV - Estimativa dos efeitos das variáveis para o parâmetro diâmetro de poros.]*

Factor Effect Standard deviation p-value Coeficient

Average 0.0575 0.0139 0.0257 0.0575

(1) Time (h) -0.0391 0.0368 0.3657 -0.0196

(2) Temperature (°C) 0.0332 0.0368 0.4331 0.0166

1 with 2 -0.0278 0.0368 0.5044 -0.0139

Table V - Estimated effects of variables for the pore volume parameter.

*[Tabela V - Estimativa dos efeitos das variáveis para o parâmetro volume de poros.]*

4.4 4.2 4.0 3.8 3.6 3.4 3.2 3.0 2.8

2.4 2.2 2.0 1.2

1.2
0.8_{0.4}

0.0_{-0.4}
-0.8_{-1.2}

-1.2 4 1.2

**T**

**e**

**m**

**p**

**e**

**ra**

**tu**

**re**

** (º**

**C**

**)**

**D**

**p**

** (n**

**m**

**)**

**Tim _{e (d}**

**ay)** **Te**

**mp**
**era**

**ture**
** (º**

**C)**

**Time (day)**

0.8

0.4 0.4

-0.8 0.0

-1.2

-1.2 -0.6 0.0 0.6 1.2 1.0

0.6

-0.6 0.2

-1.0 -0.2

4

3.2 3.2

3 3

2.8 2.8

3.8 3.8

2.6 2.6

3.6 3.6

2.4 2.4

3.4 3.4

-0.8 -0.4 0.0 0.4 0.8 2.6

Figure 3: Response surface of the variables time and temperature as a function of Dp (pore diameter).

*[Figura 3: Superfície de resposta das variáveis tempo e *
*temperatura em função do Dp (diâmetro de poros).]*

to obtain the best pore diameter conditions is shown in Fig. 3. It can be seen that smaller pore diameters are obtained by higher levels of temperature and time, as can be seen in Table II. It also agrees with the XRD patterns where it was observed that for higher levels of temperature and time, there was no formation of the mesoporous structure. In the crystallization temperature and time conditions used, pore diameters between 3.2 to 4.0 nm were obtained.

**CONCLUSIONS**

It was observed that temperature interacts negatively with crystallization time when using higher levels of both time and temperature simultaneously. The estimated effects of time and temperature variables showed no signiicant inluence on the increase of the speciic area and pore volume of the material; however, it had signiicant inluence on the pore diameter. Through the straight linear itting it was possible to obtain the mathematical model from the pore diameter of interest, to determine the optimal crystallization temperature and time values of the gel for further MCM-48 hydrothermal synthesis.

**ACKNOWLEDGEMENTS**

The authors acknowledge LCR/LABTAM/NUPPRAR (Catalysis and Reine Laboratory and Environmental Technologies Laboratory from Center of Primary Processing and Reuse of Produced Water and Waste) at Federal University of Rio Grande do Norte - UFRN and the CAPES-Brazil (Coordination for the Improvement of Higher Education Personnel) for the support of this research.

**REFERENCES**

[1] C.T. Kresge, M.E. Leonowicz, W.J. Roth, “Ordered
mesoporous molecular sieves synthesized by a liquid-crystal
template mechanism”, Nature **359** (1992) 710-712.

[2] P. Selvam, S.E. Dapurkar, “Catalytic activity of highly ordered mesoporous VMCM-48”, Appl. Catal., A: General

**276** (2004) 257-265.

[3] J.-L. Shi, Z.-L. Hua, L.-X. Zhang, “Nanocomposites from
ordered mesoporous materials”, J. Mater. Chem. **14** (2004)

795-806.

[4] X. Auvray, C. Pepipas, R. Anthore, I. Rico, A. Lattes, “X-ray study of mesophases of cetyltrimethylammonium bromide in water, formamide and glycerol”, J. Phys. Chem.

**93** (1989) 7458.

[5] S. Ren, H. Lei, L. Wang, Q. Bu, S. Chen, J. Wu, R. Ruan, “Biofuel production and kinetics analysis for microwave pyrolysis of Douglas ir sawdust pellet”, J. Anal. Appl. Pyrol.

**94 **(2012) 63-169.

[6] J.B. Parsa, M. Abassi, “Modeling and optimization of
sonochemical degradation of basic blue 41 via response
surface methodology”, J. Chem. **8**, 5 (2010) 1069-1077.
[7] D.D. Dicholkar, V.G. Gaikar, S. Kumar, R. Natarajan,
“Modeling and optimizing of steam pyrolysis of dimethyl
formamide by using response surface methodology coupled

with Box-Behnken design”, J. Anal. Appl. Pyrol. **96** (2012)

6-15.

[8] M. Arsenovic, S. Stankovic, L. Pezo, L. Manc, Z. Radojevic, “Optimization of the production process through response surface method: bricks made of loess”, Ceram. Int.

**39** (2013) 3065-3075.

[9] L.M. Costa, M.G.A. Korn, J.T. Castro, W.P.C. Santos, E.V. Carvalho, A.R.A. Nogueira, “Factorial design used for microwave-assisted digestion of bean samples”, Quim. Nova

**29 **(2006) 149-152.

[10] S.B. Bhosale, R.S. Pawade, P.K. Brahmankar, “Effect of
process parameters on MRR, TWR and surface topography in
ultrasonic machining of alumina zirconia ceramic composite”,
Ceram. Int. **40** (2014) 12831-12836.

[11] Y.F. Gomes, P.N. Medeiros, M.R.D. Bomio, I.M.G.
Santos, C.A. Paskocimas, R.M. Nascimento, F.V. Motta,
“Optimizing the synthesis of cobalt aluminate pigment using
fractional factorial design”, Ceram. Int. **41** (2015) 699-706.
[12] M.L. Felsner, C.B. Cano, J.R. Matos, L.B.
Almeida-Muradian, R.E. Bruns, “Optimization of thermogravimetric
analysis of ash content in honey”, J. Braz. Chem. Soc. **15 **

(2004) 797-802.

[13] S.J. Nejad, H. Abolghasemi, A. Moosavian, M.G.
Maragheh, “Fractional factorial design for the optimization
of supercritical carbon dioxide extraction of La3+_{, Ce}3+ _{and }

Sm3+_{ ions from a solid matrix using bis(2,4,4 trimethylpentyl)}

dithiophosphinic acid +tributylphosphate”, Chem. Eng. Res.
Des. **89**, 6 (2011) 827-835.

[14] S. Cerutti, J.A. Salonia, S.L.C. Ferreira, R.A. Olsina, L.D.
Martinez, “Factorial design for multivariate optimization of an
on-line preconcentration system for platinum determination by
ultrasonic nebulization coupled to inductively coupled plasma
optical emission spectrometry”, Talanta **63**, 4 (2004)

1077-1082.

[15] S. Cerutti, S.L.C. Ferreira, J.A. Gásquez, R.A. Olsina,
L.D. Martinez, “Optimization of the pre-concentration system
of cadmium with 1-(2-thiazolylazo)-p-cresol using a knotted
reactor and lame atomic absorption spectrometric detection”,
J. Hazard. Mater. **112** (2004) 279-283.

[16] J.A. Silva, B.P.G.L. Damasceno, F.L.H. Silva, M.S.
Madruga, D.P. Santana, “Aplicação da metodologia de
planejamento fatorial e análise de superfícies de resposta
para otimização da fermentação alcoólica’, Quim. Nova **31**, 5

(2008) 1073-1077.

[17] D.C. Montgomery, *Design and Analysis of Experiments*,

5th_{ Ed., John Wiley & Sons, New Jersey, USA (2001).}

[18] R.L. Mason, R.F. Gunst, J.L. Hess, *Statistical Design and *
*Analysis of Experiments*, 2nd_{ Ed., John Wiley & Sons, New }
Jersey, USA (2003).

[19] A. Doyle, B.K. Hodnett, “Stability of MCM-48 in aqueous solution as a function of pH”, Microporous Mesoporous Mater.

**63** (2003) 53-57.

[20] A.R. Nascimento, G.P. Figueredo, G. Rodrigues, M.A.F.
Melo, M.J.B. Souza, D.M.A. Melo, “Síntese e caracterização
de materiais mesoporosos modiicados com níquel para a
captura de CO2”, Cerâmica **60**, 356 (2014) 482-489.